Open Access on 06/05/2015
Diﬀusion NMR Study of Generation-Five PAMAM Dendrimer Materials Mallory A. van Dongen,† Bradford G. Orr,‡ and Mark M. Banaszak Holl*,†,§ †
Departments of Chemistry, ‡Department of Physics, and §Program in Macromolecular Science and Engineering, University of Michigan, 930 North University Avenue, Ann Arbor, Michigan 48109, United States ABSTRACT: Commercial generation-ﬁve poly(amidoamine) dendrimer material (G5c) was fractionated into its major structural components. Monomeric G5 (G5m; 21−30 kDa) was isolated to compare its functional properties to the G5c material. Diﬀusionordered nuclear magnetic resonance spectroscopy was employed to measure the selfdiﬀusion coeﬃcients and corresponding hydrodynamic radii of G5m and other G5c components as a function of dendrimer size (i.e., molecular weight) and tertiary structure (i.e., generational or oligomeric nature). It was found that the hydrodynamic radius (RH) scales with approximate numbers of atoms in the trailing generations, G5m, and oligomeric material at a rate of RH ∝ N0.35, in good agreement with previous reports of RH scaling for PAMAM dendrimer with generation. G5c materials can be thought of as a heterogeneous mixture of dendrimers ranging in size from trailing generation two to tetramers of G5, approximately the same in size as a G7 dendrimer, with G5m comprising ∼65% of the material. The radius of hydration for G5m was measured to be 3.1 ± 0.1 nm at pH 7.4. The 10% swelling in response to a drop in pH observed for the G5c material was not observed for isolated G5m; however, the isolated G5−G5 dimers had an increase of 44% in RH, indicating that the G5c pH response results from the increase in RH of the oligomeric fraction upon protonation. Finally, the data allow for an experimental test of the “slip” and “stick” boundary models of the Stokes−Einstein equation for PAMAM dendrimer in water.
INTRODUCTION Poly(amidoamine) (PAMAM) dendrimers have attracted signiﬁcant interest since they were ﬁrst synthesized by Tomalia et al. in 1985.1 The dendritic architecture has many properties that are interesting from both materials and biological standpoints, including the scaling of size and number of functional groups with generation. The dynamics of the branches of PAMAM dendrimers have also been shown to vary as a function of generation, with lower generations (G0− G5) being highly ﬂexible and having the ability to fold branches into the core region. For higher generations (≥G6), the branches are tightly packed and the dendrimer shape becomes more like a sphere, although backfolding of terminal groups is still observed.2,3 The primary and secondary amines of PAMAM dendrimer are protonated at diﬀerent pH levels, allowing for swelling and conformational changes as a function of pH.4−8 G5 PAMAM is particularly interesting for biological applications because of its size, which is large enough to solubilize multiple hydrophobic entities yet small enough to diﬀuse through tissue, making it an excellent scaﬀold for a variety drug and gene delivery applications.9−12 Physical properties of PAMAM dendrimer such as size and diﬀusion rate impact important biological properties including pharmacodynamics and biodistribution. Several studies have shown that molecular weight, radius, diﬀusion rates, and the density proﬁles of PAMAM all scale with generation.2,13−16 For considering biological applications, radius of hydration (RH) is a parameter of particular interest because detailed knowledge of this value is needed for understanding both diﬀusion through © 2014 American Chemical Society
and localization in biological tissue. The pH response is important as well, particularly from the range of 7.4 to 3, which is the range of tissue and cytosol to that of lysosomes. For G5 PAMAM, reported values for RH range from 2.217 to 3.47 for pH 7.4 with values as high as 4.87 nm reported under acidic conditions. This gives a reported range of hydrodynamic volume from 45 to 165 nm3 at pH 7.4 and a potential increase in volume up to 463 nm3 upon protonation in acidic media. This is a wide range of possible values at physiological pH with large consequences for expected biological properties. The dramatic volume change upon acidiﬁcation has signiﬁcant implications for the behavior of these materials in endosomes and lysosomes, where they are known to accumulate.18 Given the importance of these values for understanding key issues in drug and gene delivery, it is important to understand how the various molecular weight (MW) fractions making up commercial G5 PAMAM dendrimer contribute to the measured volumes and volume changes as a function of pH. In addition, the hydrodynamic radii and volume values for a narrow MW fraction G5 PAMAM dendrimer free of trailing generations and oligomers are desired to provide data related to the biodistribution of this fraction and for better comparison with theoretical calculations that employ ideal dendrimer structures. Most previous studies have employed unpuriﬁed Received: April 25, 2014 Revised: June 3, 2014 Published: June 5, 2014 7195
dx.doi.org/10.1021/jp504059p | J. Phys. Chem. B 2014, 118, 7195−7202
The Journal of Physical Chemistry B
Figure 1. UPLC chromatograms of commercial (black trace) and isolated fractions (overlaid colored traces). T4 appears as a left-hand shoulder to the G5m peak but cannot be isolated without substantial G5m also present.
hydrodynamic volume change of just 10%, whereas the dimer undergoes a hydrodynamic volume change of 140%. This study indicates that important physical properties relevant to biomedical application ascribed to G5 PAMAM dendrimer arise from components present as part of the mixture that makes up commercial grade G5 PAMAM material.
commercial grade materials, and this may contribute to the substantial range of values present in the literature. Recent work by van Dongen et al. indicates that as-received biomedical grade G5 PAMAM dendrimer contains ∼35% trailing and oligomeric material fractions by mass.19 The resolution of these components, which is improved as compared with many previous reports,7,20,21 was made possible by increased resolution of mass fractions using reverse-phase ultrahigh performance liquid chromatography (rp-UPLC) and a C18 column. Using these methods, the amounts of trailing generations and high oligomers were quantiﬁed. In particular, it was possible to resolve the signiﬁcant amounts of trailing generation four and dimer from the G5 monomer (G5m) PAMAM peak. The presence of trailing generations one to four (T1−T4) and dimers, trimers, and tetramers of G5 is anticipated to have a signiﬁcant impact on previous RH measurements of commercial material, including pH response. Previous measurements of G0−G3 PAMAM have indicated little size response as a function of pH, whereas materials similar in size to the oligomers, such as G6 and G7 PAMAM, are reported to have a substantially larger pH response than G5 PAMAM. In the present work, semipreparative scale reverse-phase high-performance liquid chromatography (rp-HPLC) was employed to separate commercial G5 PAMAM (G5c) material into its constituent fractions including trailing generations T1− T3, G5m (21−30 kDaA fraction, 93 −NH2 terminated arms, PDI = 1.019), and dimer, trimer, and tetramer of G5. The G5m fraction, which represents ∼65% of the as-received G5c material, contains the entire distribution of branching type defects (i.e., missing arms and intramolecular loops) with structurally perfect G5 present as